aging process
type: BFO_0000015
BFO_0000062: creep testing process 10.1016 j.msea.2008.04.097 HT1

aging process
type: BFO_0000015
BFO_0000062: creep testing process 10.1016 j.msea.2008.04.097 HT2

aging process
type: BFO_0000015
BFO_0000062: creep testing process 10.1016 j.msea.2008.04.097 HT3

chemical composition data item 10.1016 j.msea.2008.04.097 HT1
type: PMD_0025002
PMD_0000006: wt.%: C 0.04, Mn 0.09, Fe 18.64, S 0.0001, Si 0.07, Cu 0.17, Ni 53.09, Cr 18.11, Al 0.53, Ti 0.95, Co 0.21, Mo 3.03, Nb 5.05, Ta 0.01, P 0.009, B 0.003, Pb 0.1 ppm, Bi <0.1 ppm, Se <0.1 ppm, Nb + Ta 5.06

chemical composition data item 10.1016 j.msea.2008.04.097 HT2
type: PMD_0025002
PMD_0000006: wt.%: C 0.04, Mn 0.09, Fe 18.64, S 0.0001, Si 0.07, Cu 0.17, Ni 53.09, Cr 18.11, Al 0.53, Ti 0.95, Co 0.21, Mo 3.03, Nb 5.05, Ta 0.01, P 0.009, B 0.003, Pb 0.1 ppm, Bi <0.1 ppm, Se <0.1 ppm, Nb + Ta 5.06

chemical composition data item 10.1016 j.msea.2008.04.097 HT3
type: PMD_0025002
PMD_0000006: wt.%: C 0.04, Mn 0.09, Fe 18.64, S 0.0001, Si 0.07, Cu 0.17, Ni 53.09, Cr 18.11, Al 0.53, Ti 0.95, Co 0.21, Mo 3.03, Nb 5.05, Ta 0.01, P 0.009, B 0.003, Pb 0.1 ppm, Bi <0.1 ppm, Se <0.1 ppm, Nb + Ta 5.06

input specification stress 10.1016 j.msea.2008.04.097 HT1
type: PMD_0000014
IAO_0000039: MegaPA
OBI_0001937: 6.25E2
RO_0000058: quality mechanical stress 10.1016 j.msea.2008.04.097 HT1

input specification stress 10.1016 j.msea.2008.04.097 HT2
type: PMD_0000014
IAO_0000039: MegaPA
OBI_0001937: 6.25E2
RO_0000058: quality mechanical stress 10.1016 j.msea.2008.04.097 HT2

input specification stress 10.1016 j.msea.2008.04.097 HT3
type: PMD_0000014
IAO_0000039: MegaPA
OBI_0001937: 6.25E2
RO_0000058: quality mechanical stress 10.1016 j.msea.2008.04.097 HT3

input specification temperature 10.1016 j.msea.2008.04.097 HT1
type: PMD_0000014
IAO_0000039: DEG C
OBI_0001937: 6.5E2
RO_0000058: quality temperature 10.1016 j.msea.2008.04.097 HT1

input specification temperature 10.1016 j.msea.2008.04.097 HT2
type: PMD_0000014
IAO_0000039: DEG C
OBI_0001937: 6.5E2
RO_0000058: quality temperature 10.1016 j.msea.2008.04.097 HT2

input specification temperature 10.1016 j.msea.2008.04.097 HT3
type: PMD_0000014
IAO_0000039: DEG C
OBI_0001937: 6.5E2
RO_0000058: quality temperature 10.1016 j.msea.2008.04.097 HT3

manufacturing process
type: BFO_0000015
BFO_0000062: creep testing process 10.1016 j.msea.2008.04.097 HT1

manufacturing process
type: BFO_0000015
BFO_0000062: creep testing process 10.1016 j.msea.2008.04.097 HT2

manufacturing process
type: BFO_0000015
BFO_0000062: creep testing process 10.1016 j.msea.2008.04.097 HT3

material identifier 10.1016 j.msea.2008.04.097 HT1
type: MWO_0001099
IAO_0000219: creep test piece 10.1016 j.msea.2008.04.097 HT1
PMD_0000006: Inconel 718

material identifier 10.1016 j.msea.2008.04.097 HT2
type: MWO_0001099
IAO_0000219: creep test piece 10.1016 j.msea.2008.04.097 HT2
PMD_0000006: Inconel 718

material identifier 10.1016 j.msea.2008.04.097 HT3
type: MWO_0001099
IAO_0000219: creep test piece 10.1016 j.msea.2008.04.097 HT3
PMD_0000006: Inconel 718

object identifier 10.1016 j.msea.2008.04.097 HT1
type: MWO_0001015
IAO_0000219: creep test piece 10.1016 j.msea.2008.04.097 HT1
PMD_0000006: HT1

object identifier 10.1016 j.msea.2008.04.097 HT2
type: MWO_0001015
IAO_0000219: creep test piece 10.1016 j.msea.2008.04.097 HT2
PMD_0000006: HT2

object identifier 10.1016 j.msea.2008.04.097 HT3
type: MWO_0001015
IAO_0000219: creep test piece 10.1016 j.msea.2008.04.097 HT3
PMD_0000006: HT3

standard 10.1016 j.msea.2008.04.097 HT1
type: NFDI_0000206
RO_0000058: plan 10.1016 j.msea.2008.04.097 HT1
PMD_0000006: ASTM E 8M-94a

standard 10.1016 j.msea.2008.04.097 HT2
type: NFDI_0000206
RO_0000058: plan 10.1016 j.msea.2008.04.097 HT2
PMD_0000006: ASTM E 8M-94a

standard 10.1016 j.msea.2008.04.097 HT3
type: NFDI_0000206
RO_0000058: plan 10.1016 j.msea.2008.04.097 HT3
PMD_0000006: ASTM E 8M-94a

Aging
type: NFDI_0001018
IAO_0000219: aging process
PMD_0000006: 955 C, 1 h/AC + 720 C, 8 h/FC 57 K/h to 620 C, 8 h/AC

Aging
type: NFDI_0001018
IAO_0000219: aging process
PMD_0000006: no aging condition 955 C

Aging
type: NFDI_0001018
IAO_0000219: aging process
PMD_0000006: 955 C, 3.5 h/AC

Processing method
type: NFDI_0001018
IAO_0000219: manufacturing process
PMD_0000006: DUVAC (VIM electrode and VAR ingot) processes

Processing method
type: NFDI_0001018
IAO_0000219: manufacturing process
PMD_0000006: DUVAC (VIM electrode and VAR ingot) processes

Processing method
type: NFDI_0001018
IAO_0000219: manufacturing process
PMD_0000006: DUVAC (VIM electrode and VAR ingot) processes

Solutionizing
type: NFDI_0001018
IAO_0000219: solutionizing process 10.1016 j.msea.2008.04.097 HT1
PMD_0000006: 1095 C, 1 h/AC

Solutionizing
type: NFDI_0001018
IAO_0000219: solutionizing process 10.1016 j.msea.2008.04.097 HT2
PMD_0000006: 1095 C, 1 h/AC

Solutionizing
type: NFDI_0001018
IAO_0000219: solutionizing process 10.1016 j.msea.2008.04.097 HT3
PMD_0000006: 1095 C, 1 h/AC

value specification creep rupture time 10.1016 j.msea.2008.04.097 HT1
type: OBI_0001931
OBI_0001927: stress rupture time 10.1016 j.msea.2008.04.097 HT1
OBI_0002135: 159.74 ±19.18 h

value specification creep rupture time 10.1016 j.msea.2008.04.097 HT2
type: OBI_0001931
OBI_0001927: stress rupture time 10.1016 j.msea.2008.04.097 HT2
OBI_0002135: 331.18 ±28.93 h

value specification creep rupture time 10.1016 j.msea.2008.04.097 HT3
type: OBI_0001931
OBI_0001927: stress rupture time 10.1016 j.msea.2008.04.097 HT3
OBI_0002135: 196.75 ±16.48 h

value specification grain size 10.1016 j.msea.2008.04.097 HT1
type: OBI_0001931
IAO_0000039: MicroM
OBI_0001927: quality grain size 10.1016 j.msea.2008.04.097 HT1
OBI_0001937: 1.7E2

value specification grain size 10.1016 j.msea.2008.04.097 HT2
type: OBI_0001931
IAO_0000039: MicroM
OBI_0001927: quality grain size 10.1016 j.msea.2008.04.097 HT2
OBI_0001937: 1.6E2

value specification grain size 10.1016 j.msea.2008.04.097 HT3
type: OBI_0001931
IAO_0000039: MicroM
OBI_0001927: quality grain size 10.1016 j.msea.2008.04.097 HT3
OBI_0001937: 1.55E2

value specification percentage elongation after creep fracture 10.1016 j.msea.2008.04.097 HT1
type: OBI_0001931
OBI_0001927: quality percentage elongation after creep fracture 10.1016 j.msea.2008.04.097 HT1
OBI_0002135: 1.1542 ±0.0577%

value specification percentage elongation after creep fracture 10.1016 j.msea.2008.04.097 HT2
type: OBI_0001931
OBI_0001927: quality percentage elongation after creep fracture 10.1016 j.msea.2008.04.097 HT2
OBI_0002135: 5.3565 ±0.2678%

value specification percentage elongation after creep fracture 10.1016 j.msea.2008.04.097 HT3
type: OBI_0001931
OBI_0001927: quality percentage elongation after creep fracture 10.1016 j.msea.2008.04.097 HT3
OBI_0002135: 1.4892 ±0.0745%

value specification steady state creep rate 10.1016 j.msea.2008.04.097 HT1
type: OBI_0001931
OBI_0001927: quality creep rate 10.1016 j.msea.2008.04.097 HT1
OBI_0002135: 0.96 ×10−4 ±5.16×10−6

value specification steady state creep rate 10.1016 j.msea.2008.04.097 HT2
type: OBI_0001931
OBI_0001927: quality creep rate 10.1016 j.msea.2008.04.097 HT2
OBI_0002135: 1.42 ×10−4 ±2.05 ×10−6

value specification steady state creep rate 10.1016 j.msea.2008.04.097 HT3
type: OBI_0001931
OBI_0001927: quality creep rate 10.1016 j.msea.2008.04.097 HT3
OBI_0002135: 1.04 ×10−4 ±3.49 ×10−6